IOSR Journal of Applied Physics (IOSR-JAP) e-ISSN: 2278-4861. Volume 6, Issue 1 Ver. I (Jan. 2014), PP 42-46 www.iosrjournals.org
Investigation on the Linear and Nonlinear Optical Properties of L-Lysine Doped Ammonium Dihydrogen Phosphate Crystal for NLO Applications R.N. Shaikh1, Mohd.Anis1, M.D. Shirsat2 and S.S. Hussaini1* 1
Crystal Growth Laboratory, Department of Physics, Milliya Arts, Science and Management Science College, Beed-431122, Maharashtra, India. 2 Intelligent Materials Research Laboratory, Department of Physics, Dr. Babasaheb Ambedkar Marathwada University, Aurangabad-431004, Maharashtra, India.
Abstract : In present investigation L-lysine doped ADP crystal has been grown by slow evaporation technique. The crystalline nature of the grown crystal was confirmed using powder X-ray diffraction technique. The optical studies were carried to examine optical transparency and determine the optical constants of the grown crystal quenching the optoelectronics applications. The optical band gap of grown crystal is found to be 4.7eV. The third order nonlinear behaviour has been investigated using Z-scan technique at 632.8 nm. The nonlinear third order susceptibility of grown crystal is found to be 1 .578 x 10-5 esu. The nonlinear index of refraction and absorption coefficient were determined to explore the optical limiting applications of the grown NLO crystal. The kurtz powder test confirmed the second harmonic generations by the grown crystal. Keywords: Growth from solution; UV-Vis; Optical properties; optical susceptibility; SHG efficiency. I. Introduction Nonlinear optical (NLO) frequency conversion materials have a significant impact on laser technology, optical communication and optical storage technology. Ammonium dihydrogen phosphate (ADP) is a potential inorganic material having wide range of applications such as electro-optic modulator, harmonic generators and parametric generators [1-5]. The amino acids are organic materials for NLO application as they have donor carboxylic (COOH) group and the proton acceptor (NH2) amino group, known as zwitter-ions. Therefore, amino acids can be used as dopants and it was observed that there is enhancement in the material properties such as NLO and ferroelectric properties . L-lysine posses a side chain with hydrogen atom which offers to charge transfer to form semiorganic crystals for nonlinear optical applications . In literature anisotropic studies of L-alanine, glycine, L-arginine and DL-malik acid doped ADP crystal has been reported [8-10]. The influence of L-lysine monohydrochloride dihydrate on the growth and properties of ADP single crystal have been reported by P. Rajesh et al. . However, no reports on linear and nonlinear properties of L-lysine doped ADP crystal were found. Thus present study reports detailed evaluation of optical properties (optical band gap, extinction coefficient, refractive index, optical conductivity) and third order nonlinear coefficients of L-lysine doped ADP crystal for possible application in optical limiting devices.
The AR grade ADP salt was dissolved in deionised water with constant stirring to achieve the supersaturated solution. The saturated solution of ADP was added with 1, 2 and 3 mole percent of L-lysine separately. The L-lysine added solutions were allowed to stir at constant speed to achieve the homogeneity throughout the volume. The Prepared solutions were then filtered and the purity of the salts was achieved by repetitive recrystallization, good quality transparent seed crystals were harvested within 5-6 days by slow evaporation method at room temperature. The Synthesized salts of 1, 2 and 3 mole% L-lysine doped ADP were subjected to SHG test, and it was observed that the 2 mole% L-lysine doped ADP crystal exhibited more SHG efficiency as compare to 1 & 3 mole % and hence of 2 mole% L-lysine doped ADP crystal was grown by slow evaporation technique. The grown crystal is shown in Fig 1.
42 | Page
Investigation on the Linear and Nonlinear Optical Properties of L-Lysine Doped Ammoniu
Fig 1. Photograph of the 2 mole% L-lysine doped ADP crystal III.
Results And Discussion
3.1. X-ray Diffraction Analysis The grown crystal was subjected to powder XRD and the pattern is shown in Fig 2, the unit cell parameters obtained are a=b=7.504 A0 and c=7.588 A0 α=β=γ=900. The obtained lattice parameter values are in good agreement with literature .
Fig 2. Indexed pattern of doped ADP
Fig 3. UV-Vis. Transmittance Spectrum
3.2 NLO STUDIES The second harmonic generation of the grown crystals was examined using the Kurtz and Perry powder technique . The salts of 1,2 and 3mole percent L-lysine doped ADP were subjected to SHG test at IISC, Bangalore, The wavelength 1064 nm from a Q-switched Nd: YAG laser with a pulse energy 2.8mJ/pulse, pulse width 8 ns, and repetition rate of 10 Hz was used. The collected green emission from the powdered sample at the output confirmed the nonlinear behavior of 1, 2 and 3 mole % L-lysine doped ADP crystal. But the 2 mole% L-lysine doped ADP crystal has high output as compare to 1 & 3 mole % L-lysine doped ADP. 3.3 OPTICAL STUDIES The UV-Visible spectral study of 2 mole % L-lysine doped ADP crystal was carried out using Shimadzu UV-2450 Spectrophotometer in the range 200-900 nm and the recorded transmittance is shown in Fig 3. The grown crystal exhibits high transmittance above 85% in entire visible region. The lower cutoff wavelength is found to be 260 nm indicating the wide optical transmission window favorable for second harmonic generation . The dependence of the optical absorption coefficient (α) on the photon energy (hν) used to study the band structure and the types of transitions of electrons. The electronic band transitions can be well understood from the plot of (αhν) 2 verses photon energy as depicted in Fig 4. The wide optical band gap of doped ADP crystal is found to be 4.7 eV suggesting its suitability for optoelectronics applications . www.iosrjournals.org
43 | Page
Investigation on the Linear and Nonlinear Optical Properties of L-Lysine Doped Ammoniu The variations of extinction coefficient, refractive index are sequentially shown in Fig 5& 6. The least absorption and significantly lower index of refraction in entire visible region exhibited by doped ADP crystal is most desirable property for antireflection coating in solar thermal devices . The plot of optical conductivity against the photon energy is shown in Fig 7. The higher photonic response of optical conductivity and low extinction coefficient is of vital importance for applications in information processing and computing devices. Thus doped ADP crystal is prominent material for NLO applications .
Fig.4 ( h )2 vs. photon energy (hν)
Fig 5. Extinction coefficient vs. Wavelength
Fig 6. Refractive index vs. wavelength
Fig 7. Optical conductivity vs. Photon Energy
3.4 Z-SCAN STUDIES The single-beam Z-scan is a well-known technique to evaluate the third order nonlinear optical properties of the materials. It allows the simultaneous measurement of both the nonlinear refractive index and nonlinear absorption coefficient. The study of nonlinear refraction by the Z-scan method is based on the intensity dependence of the crystal along a focused Gaussian laser beam. The positive nonlinear refraction or the defocusing due to a negative refraction can be studied using closed aperture transmittance data . A Gaussian beam is focused by a spherical lens onto the sample using a lens of focal length 21.5 cm placed at a far field. The sample is moved along the Z direction and by monitoring the transmittance variation through a small aperture placed at the far ﬁeld position. The open aperture transmittance data was recorded to determine the nonlinear absorption coefficient of the material. The difference between the peak and valley transmission (ΔTpv) is written in terms of the on axis phase shift at the focus as,
Tp v 0.406(1 S )0.25
where S is the aperture linear transmittance and is calculated using the relation
S 1 exp(2ra 2 / a 2 )
where ra is the aperture and ωa is the beam radius at the aperture. The nonlinear refractive index is given by
KI 0 Leff
Where K = 2π / λ (λ is the laser wavelength), I0 is the intensity of the laser beam at the focus (Z=0), www.iosrjournals.org
44 | Page
Investigation on the Linear and Nonlinear Optical Properties of L-Lysine Doped Ammoniu Leff = [1- exp (-αL)]/ α is the effective thickness of the sample, α is the linear absorption and L is the thickness of the sample. From the open aperture Z-scan data, the nonlinear absorption coefficient is estimated as
2 2T I 0 Leff
where ΔT is the one valley value at the open aperture Z-scan curve. The value of β will be negative for saturable absorption and positive for two photon absorption. The real and imaginary parts of the third order nonlinear optical susceptibility χ (3) are defined as
Re (3) (esu) 104 ( 0C 2 n0 2 n2 ) / (cm2 / W )
Im (esu) 10 ( 0C n0 ) / 4 (cm / W )
where ε0 is the vacuum permittivity, n0 is the linear refractive index of the sample and c is the velocity of light in vacuum.
Table 1.Measurement details and the results of the Z-scan technique Laser beam wavelength (λ) Lens focal length (f) Optical path distance (Z) Spot-size diameter in front of the aperture (ωa) Aperture radius (ra) Incident intensity at the focus (Z=0) Effective thickness Leff Linear absorption coefficient Nonlinear refractive index (n2) Nonlinear absorption coefficient (β) Third-order nonlinear optical susceptibility (χ3)
632.8 nm 12 cm 115 cm 1 cm 4 mm 3.13 MW/Cm2 1.804 mm 1.103 - 2.68 x10-13cm /W 4.063 x 10-6 cm/W 1.578 x 10-5 esu
Thus, we can easily obtain the absolute value of χ3 by the following formula
3 (Re 3 )2 (Im 3 )2
The closed aperture transmittance data depicted in Fig 8 confirms the self defocusing nature as prefocal transmittance peak is followed by the postfocal transmittance valley, indicating negative index of refraction. The negative index of refraction of doped ADP crystal makes it prominent material for protection optical night vision sensor devices . The nonlinear refractive index is found to be - 2.68 x10-13 cm /W. The open aperture transmittance data confirmed the saturable absorption by the doped ADP crystal depicted in Fig 9. The open aperture transmittance data was employed to evaluate the nonlinear absorption coefficient (β) of the grown crystal. The effective β value of doped ADP crystal is found to be 4.063 x 10 -6 cm/W which is relatively lower than potential NLO material . The nonlinear third order susceptibility of grown crystal is found to be 1.578 x 10-5esu which is notably greater than reported crystals . The figure of merit (FOM) can be evaluated using the relation (βλ/n2). The FOM value of grown crystal is found to be 0.0959 indicating its suitability for photonics applications . The promising third order NLO properties of doped ADP crystals are discussed in Table 1, suggesting its suitability for applications in optical limiting and photonics devices.
Fig 8. Closed aperture Z-Scan curve
Fig 9. Open aperture Z-Scan curve www.iosrjournals.org
45 | Page
Investigation on the Linear and Nonlinear Optical Properties of L-Lysine Doped Ammoniu IV. Conclusions The L-lysine doped ADP crystal has been grown from aqueous solution by slow evaporation technique at room temperature. The kurtz powder test confirmed the second harmonic generation of the grown crystal. The optical studies showed wide optical transparency window and enhanced optical constants essential for optoelectronics applications. The optical band gap was found to be 4.7 eV. The negative refractive index ascertained the self-defocusing nature, which is prerequisite property for optical limiting application. The significantly lower nonlinear absorption, FOM value and higher third order susceptibility of grown crystal makes it promising material for integrated NLO applications.
Acknowledgments The authors are thankful to the Department of Science and Technology (DST/SR/S2/LOP-22/2010), and University Grants Commission (UGC/41-591/2012/SR), New Delhi, for financial assistance. The authors are also thankful to Prof. P.K Das, Department of Physical Chemistry, Indian Institute of Science (IISc), Bangalore, India for SHG Test. Also the authors would like to thank Prof. D. Sastikumar, Department of Physics, National Institute of Technology, Tirucherapalli, India for extending the facility for Z-scan measurement.
References   
      
        
N.R. Dhumane, S.S. Hussaini, V.G. Dongre, P. Ghugare, M.D. Shirsat, Growth and characterization of L-Alanine-doped Zinc Thiourea Chloride single crystal (ZTC), Applied Physics A, 95, 2009, 727-732. P. Rajesh, P. Ramasamy, Optical, dielectric and microhardness studies on (100) directed ADP crystal, Spectrochimica Acta part A, 74, 2009, 210-213. S.S. Hussaini, N.R. Dhumane, V.G. Dongre, P. Karmuse, P. Ghughare, M.D. Shirsat, Effect of Glycine on the optical properties of Zinc Thiourea Chloride single crystal, Journal of Optoelectronics and Advanced Material (Rapid Communication), 2, 2008, 108112. K. Meera, R. Muralidharan, R. Dhanasekaran, M. Prapun, P. Ramasamy, Growth of nonlinear optical material: L-arginine hydrochloride and its characterization, Journal of Crystal Growth, 263, 2004, 510-516. N.R. Dhumane, S.S. Hussaini, V.G. Dongre, Mahendra D. Shirsat, InďŹ‚uence of glycine on the nonlinear optical (NLO) properties of zinc (tris) thiourea sulfate (ZTS) single crystal, Optical Materials, 31, 2008, 328-332. N.R. Dhumane, S.S. Hussaini, V.G. Dongre, P.P. Karmuse, and M.D. Shirsat, Growth and characterization of glycine doped bisthiourea cadmium chloride single crystal, Journal of Crystal Research Technology, 44, 2009, 269-274. R. Ramesh Babu, N. Vijayan, R. Gopalakrishnan, P.Ramasamy, Growth and characterization of L-lysine monohydrochloride dihydrate (L-LMHCl) single crystal, Crystal Research Technology 41,2006, 405-410. Ferdousi Akhtar, Jiban Podder, Structural,Optical,Electrical and Thermal Characterizations of Pure & L-alanine Doped Ammonium Dihydrogen Phosphate Crystals, Journal of Crystallisation Process & Technology, 1, 2011, 18-25. P. Rajesh, P. Ramasamy, Growth of DL-malic acid-doped ammonium dihydrogen phosphate crystal and its Characterization, Journal of Crystal Growth, 311, 2009, 3491-3497. N. Pattanaboonmee, P.Ramaswamy, R.Yimnirun, P.Manyum, A comparative study on pure, L-arginine and glycine doped ammonium dihydrogen orthophosphate single crystals grown by slow evaporation and temperature-gradient method, Journal of Crystal Growth, 314, 2011, 196-201. P.Rajesh, P.Ramasamy, C.K. Mahadevan, Effect of L-lysine monohydrochloride dihydrate on the growth and properties of ammonium dihydrogen orthophosphate single crystals, Journal of Crystal Growth, 311, 2009, 1156-1160. S.K. Kurtz, T.T. Perry, A Powder technique for the evaluation of Nonlinear Optical Materials, Journal of Applied Physics,39(8), 1968, 3798-3813. R. Santhakumari , K. Ramamurthi, Structural, thermal and optical characterization of an organic NLO Material-Benzaldehyde thiosemicarbazone monohydrate single crystals, Spectrochimica Acta part A, 78, 2011, 653-659. D. Kalaiselvi, R. Jayavel, Synthesis, growth and characterization of L-proline dimercuricchloride single crystals for frequency conversion applications, Applied Physics A, 107, 2012, 93-100. T. C. Sabari Girisun, S. Dhanuskodi, Linear and nonlinear optical properties of tris thiourea zinc sulphate single crystals, Journal of Crystal Research Technology, 44,2009, 1297- 1302. S. Dhanuskodi, A. Philominal, J. Philip, K. Kim, J. Yi, Optical and dielectric properties of nitrophenolate based nonlinear optical crystal, Journal of Material Science 46, 2011, 3169-3175. P.V. Dhanaraj, N.P. Rajesh, Investigations on crystal growth, structural, optical, dielectric, mechanical and thermal properties of a novel optical crystal: Nicotinium nitrate monohydrate, Journal of Crystal Growth 318, 2011, 974-978. G. Pabitha, R. Dhanasekaran, Investigation on the linear and nonlinear optical properties of a metal organic complexâ€”Bis thiourea zinc acetate single crystal, Optics & Laser Technology, 50, 2013, 150-154. P.T. Anusha, P. Silviya Reeta, L. Giribabu, S.P. Tewari, S. Venugopal Rao, Picosecond nonlinear optical studies of unsymmetrical alkyl and alkoxy phthalocyanine, Materials Letters, 64, 2010, 1915-1917.
46 | Page